LMucko/crystallography-open-database huggingface dataset:
Crystal structure of dehydrated potassium-exchanged zeolite A. Absence of supposed zero-coordinated potassium. Refinement of Si, Al-ordered superstructure
Pluth, J.J.; Smith, J.V.; Journal of Physical Chemistry 83 (1979) 741–749; doi:

data_1530598
_publ_section_title
;
 Crystal structure of dehydrated potassium-exchanged zeolite A. Absence of
 supposed zero-coordinated potassium. Refinement of Si, Al-ordered
 superstructure
;
_journal_name_full               'Journal of Physical Chemistry'
_journal_page_first              741
_journal_page_last               749
_journal_volume                  83
_journal_year                    1979
_chemical_formula_sum            'Al12 K11.41 O48 Si12'
_chemical_name_systematic        'K11.41 (Al12 Si12 O48)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   12.3
_cell_length_b                   12.3
_cell_length_c                   12.3
_cell_volume                     1860.867
_citation_journal_id_ASTM        JPCHAX
_cod_data_source_file            Pluth_JPCHAX_1979_451.cif
_cod_data_source_block           Al12K11.41O48Si12
_cod_database_code               1530598
About the crystal structure of eudidymite Na Be Si3 O7 O H
Pobedimskaya, E.A.; Belov, N.V.; Doklady Akademii Nauk SSSR 136 (1961) 1448–1450; doi:

data_1530599
_publ_section_title
;
 About the crystal structure of eudidymite Na Be Si3 O7 O H
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              1448
_journal_page_last               1450
_journal_volume                  136
_journal_year                    1961
_chemical_formula_sum            'Be H Na O8 Si3'
_chemical_name_systematic        'Na Be (Si3 O7) (O H)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 103.75
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.63
_cell_length_b                   7.38
_cell_length_c                   14.02
_cell_volume                     1269.346
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Pobedimskaya_DANKAS_1961_551.cif
_cod_data_source_block           H1Be1Na1O8Si3
_cod_original_formula_sum        'H1 Be1 Na1 O8 Si3'
_cod_database_code               1530599
Refined crystal structures of gamma-La2 S3 and gamma-Sm2 S3. Ratio of the Th3 P4 and zircon structures
Podberezskaya, N.V.; Kozhemyak, N.V.; Golubeva, L.G.; Bakakin, V.V.; Balko, V.P.; Borisov, S.V.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 20 (1979) 1092–1095; doi:

data_1530600
_publ_section_title
;
 Refined crystal structures of gamma-La2 S3 and gamma-Sm2 S3. Ratio of the
 Th3 P4 and zircon structures
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              1092
_journal_page_last               1095
_journal_volume                  20
_journal_year                    1979
_chemical_formula_sum            'La10.68 S16'
_chemical_name_systematic        '(La2 S3)5.24'
_space_group_IT_number           220
_symmetry_space_group_name_Hall  'I -4bd 2c 3'
_symmetry_space_group_name_H-M   'I -4 3 d'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   8.692
_cell_length_b                   8.692
_cell_length_c                   8.692
_cell_volume                     656.688
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Podberezskaya_ZSTKAI_1979_690.cif
_cod_data_source_block           La10.68S16
_cod_original_cell_volume        656.6882
_cod_database_code               1530600
A new form of the Scheelite structural type: crystal structure of Nd2 W O6
Polyanskaya, T.M.; Borisov, S.V.; Belov, N.V.; Doklady Akademii Nauk SSSR 193 (1970) 83–86; doi:

data_1530601
_publ_section_title
;
 A new form of the Scheelite structural type: crystal structure of Nd2 W
 O6
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              83
_journal_page_last               86
_journal_volume                  193
_journal_year                    1970
_chemical_formula_sum            'Nd2 O6 W'
_chemical_name_systematic        'Nd2 W O6'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-I 2yc'
_symmetry_space_group_name_H-M   'I 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 92
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   15.92
_cell_length_b                   11.39
_cell_length_c                   5.508
_cell_volume                     998.151
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Polyanskaya_DANKAS_1970_708.cif
_cod_data_source_block           Nd2O6W1
_cod_original_cell_volume        998.1506
_cod_original_sg_symbol_Hall     '-C 2yc (x,y,-x+z)'
_cod_original_formula_sum        'Nd2 O6 W1'
_cod_database_code               1530601
The crystal structure of cobalt sulfate hexacarbamide
Ponomarenko, V.I.; Kurkutova, E.N.; Porai-Koshits, M.A.; Sulaimankulov, K.; Doklady Akademii Nauk SSSR 234 (1977) 1074–1077; doi:

data_1530602
_publ_section_title
;
 The crystal structure of cobalt sulfate hexacarbamide
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              1074
_journal_page_last               1077
_journal_volume                  234
_journal_year                    1977
_chemical_formula_sum            'C6 H26 Co N12 O11 S'
_chemical_name_systematic        'Co (O C (N H2)2)6 (H2 O) S O4'
_space_group_IT_number           29
_symmetry_space_group_name_Hall  'P 2c -2ac'
_symmetry_space_group_name_H-M   'P c a 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   15.073
_cell_length_b                   7.215
_cell_length_c                   20.045
_cell_volume                     2179.928
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Ponomarenko_DANKAS_1977_218.cif
_cod_data_source_block           C6H26Co1N12O11S1
_cod_original_formula_sum        'C6 H26 Co1 N12 O11 S1'
_cod_database_code               1530602
The crystal structure of cerium (III) sulfate-2-urea-5-water Ce2 (S O4)3 (O C (N H2)2)2 (H2 O)5 and the structural characteristics of the sulfates of the rare earth elements
Ponomarenko, V.I.; Porai-Koshits, M.A.; Kurkutova, E.N.; Sulaimankulov, K.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 19 (1978) 856–865; doi:

data_1530603
_publ_section_title
;
 The crystal structure of cerium (III) sulfate-2-urea-5-water Ce2 (S O4)3
 (O C (N H2)2)2 (H2 O)5 and the structural characteristics of the sulfates
 of the rare earth elements
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              856
_journal_page_last               865
_journal_volume                  19
_journal_year                    1978
_chemical_formula_sum            'C2 H18 Ce2 N4 O19 S3'
_chemical_name_systematic        'Ce2 (S O4)3 (O C (N H2)2)2 (H2 O)5'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                85.5
_cell_angle_beta                 92.23
_cell_angle_gamma                104.98
_cell_formula_units_Z            2
_cell_length_a                   11.097
_cell_length_b                   13.409
_cell_length_c                   6.83
_cell_volume                     978.554
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Ponomarenko_ZSTKAI_1978_1368.cif
_cod_data_source_block           C2H18Ce2N4O19S3
_cod_original_cell_volume        978.5543
_cod_database_code               1530603
Crystal structure of tetracalcium trihydrotrialuminate C4 A3 H3
Ponomarev, V.I.; Kheiker, D.M.; Belov, N.V.; Doklady Akademii Nauk SSSR 194 (1970) 1072–1075; doi:

data_1530604
_publ_section_title
;
 Crystal structure of tetracalcium trihydrotrialuminate C4 A3 H3
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              1072
_journal_page_last               1075
_journal_volume                  194
_journal_year                    1970
_chemical_formula_sum            'Al3 Ca2 H3 O8'
_chemical_name_systematic        'Ca2 (Al O2)3 (O H) (H2 O)'
_space_group_IT_number           64
_symmetry_space_group_name_Hall  '-A 2ab 2ab'
_symmetry_space_group_name_H-M   'A b m a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   12.426
_cell_length_b                   12.809
_cell_length_c                   8.864
_cell_volume                     1410.835
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Ponomarev_DANKAS_1970_719.cif
_cod_data_source_block           H3Al3Ca2O8
_cod_original_sg_symbol_Hall     '-C 2ac 2 (z,x,y)'
_cod_original_formula_sum        'H3 Al3 Ca2 O8'
_cod_database_code               1530604
The crystal structure of Ba Ge O3 H2 O
Ponomarev, V.I.; Filipenko, O.S.; Pobedimskaya, E.A.; Belov, N.V.; Doklady Akademii Nauk SSSR 215 (1974) 584–587; doi:

data_1530605
_publ_section_title
;
 The crystal structure of Ba Ge O3 H2 O
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              584
_journal_page_last               587
_journal_volume                  215
_journal_year                    1974
_chemical_formula_sum            'Ba Ge H2 O4'
_chemical_name_systematic        'Ba (Ge O3) (H2 O)'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                91.167
_cell_angle_beta                 92.75
_cell_angle_gamma                89.833
_cell_formula_units_Z            4
_cell_length_a                   7.48
_cell_length_b                   7.7
_cell_length_c                   7.16
_cell_volume                     411.826
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Ponomarev_DANKAS_1974_778.cif
_cod_data_source_block           H2Ba1Ge1O4
_cod_original_cell_volume        411.8262
_cod_original_formula_sum        'H2 Ba1 Ge1 O4'
_cod_database_code               1530605
Structure and lattice dynamics of Sb Nb O4 crystals at 300-1000 K
Ponomarev, V.I.; Filipenko, O.S.; Venevtsev, Yu.N.; Ivanov, S.A.; Atovmyan, L.O.; Rannev, N.V.; Kristallografiya 26 (1981) 341–348; doi:

data_1530606
_publ_section_title
;
 Structure and lattice dynamics of Sb Nb O4 crystals at 300-1000 K
;
_journal_name_full               Kristallografiya
_journal_page_first              341
_journal_page_last               348
_journal_volume                  26
_journal_year                    1981
_chemical_formula_sum            'Nb O4 Sb'
_chemical_name_systematic        'Sb (Nb O4)'
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P 2c -2n'
_symmetry_space_group_name_H-M   'P n a 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.557
_cell_length_b                   4.932
_cell_length_c                   11.795
_cell_volume                     323.267
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Ponomarev_KRISAJ_1981_1962.cif
_cod_data_source_block           Nb1O4Sb1
_cod_original_cell_volume        323.2671
_cod_original_formula_sum        'Nb1 O4 Sb1'
_cod_database_code               1530606
About the crystal structure of potassium tetranitropalladate
Porai-Koshits, M.A.; Doklady Akademii Nauk SSSR 58 (1947) 603–605; doi:

data_1530607
_publ_section_title
;
 About the crystal structure of potassium tetranitropalladate
;
_journal_name_full               'Doklady Akademii Nauk SSSR'
_journal_page_first              603
_journal_page_last               605
_journal_volume                  58
_journal_year                    1947
_chemical_formula_sum            'K2 N4 O8 Pd'
_chemical_name_systematic        'K2 (Pd (N O2)4)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 96.57
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.82
_cell_length_b                   12.82
_cell_length_c                   9.44
_cell_volume                     940.168
_citation_journal_id_ASTM        DANKAS
_cod_data_source_file            Porai-Koshits_DANKAS_1947_1973.cif
_cod_data_source_block           K2N4O8Pd1
_cod_original_cell_volume        940.1675
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'K2 N4 O8 Pd1'
_cod_database_code               1530607
Crystal structure of potassium tetranitroplatinate
Porai-Koshits, M.A.; Kukina, G.A.; Nikolaev, V.P.; Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR)) 4 (1978) 1435–1440; doi:

data_1530608
_publ_section_title
;
 Crystal structure of potassium tetranitroplatinate
;
_journal_name_full
;
Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR))
;
_journal_page_first              1435
_journal_page_last               1440
_journal_volume                  4
_journal_year                    1978
_chemical_formula_sum            'K2 N4 O8 Pt'
_chemical_name_systematic        'K2 (Pt (N O2)4)'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 95.93
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.771
_cell_length_b                   12.795
_cell_length_c                   9.219
_cell_volume                     911.740
_citation_journal_id_ASTM        KOKHDC
_cod_data_source_file            Porai-Koshits_KOKHDC_1978_633.cif
_cod_data_source_block           K2N4O8Pt1
_cod_original_cell_volume        911.7396
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'K2 N4 O8 Pt1'
_cod_database_code               1530608
Rare-earth trisulfimidates. Crystal structure of (H2 O)6 Nd (O2 S N)3
Porai-Koshits, M.A.; Sokol, V.I.; Kop'eva, M.A.; Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR)) 8 (1982) 702–708; doi:

data_1530609
_publ_section_title
;
 Rare-earth trisulfimidates. Crystal structure of (H2 O)6 Nd (O2 S N)3
;
_journal_name_full
;
Koordinatsionnaya Khimiya (= Coordination Chemistry (USSR))
;
_journal_page_first              702
_journal_page_last               708
_journal_volume                  8
_journal_year                    1982
_chemical_formula_sum            'H12 N3 Nd O12 S3'
_chemical_name_systematic        'Nd (O2 S N)3 (H2 O)6'
_space_group_IT_number           155
_symmetry_space_group_name_Hall  'R 3 2"'
_symmetry_space_group_name_H-M   'R 3 2 :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   10.514
_cell_length_b                   10.514
_cell_length_c                   19.987
_cell_volume                     1913.437
_citation_journal_id_ASTM        KOKHDC
_cod_data_source_file            Porai-Koshits_KOKHDC_1982_890.cif
_cod_data_source_block           H12N3Nd1O12S3
_cod_original_formula_sum        'H12 N3 Nd1 O12 S3'
_cod_database_code               1530609
The structure of the crystals of salt platinum trans-dichlorodiammine
Porai-Koshits, M.A.; Trudy Instituta Kristallografii, Akademiya Nauk SSSR 9 (1954) 229–238; doi:

data_1530610
_publ_section_title
;
 The structure of the crystals of salt platinum trans-dichlorodiammine
;
_journal_name_full
'Trudy Instituta Kristallografii, Akademiya Nauk SSSR'
_journal_page_first              229
_journal_page_last               238
_journal_volume                  9
_journal_year                    1954
_chemical_formula_sum            'Cl2 H6 N2 Pt'
_chemical_name_systematic        '(N H3)2 Cl2 Pt'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 93.75
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.07
_cell_length_b                   6.05
_cell_length_c                   5.46
_cell_volume                     266.006
_citation_journal_id_ASTM        TIKRAS
_cod_data_source_file            Porai-Koshits_TIKRAS_1954_1880.cif
_cod_data_source_block           H6Cl2N2Pt1
_cod_original_cell_volume        266.0056
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_original_formula_sum        'H6 Cl2 N2 Pt1'
_cod_database_code               1530610
Crystal Structure of Praseodymium oxide iodide
Potapova, O.G.; Vasil'eva, I.G.; Borisov, S.V.; Zhurnal Strukturnoi Khimii (Issue-No. from 1981) 18 (1977) 573–577; doi:

data_1530611
_publ_section_title
;
 Crystal Structure of Praseodymium oxide iodide
;
_journal_name_full
'Zhurnal Strukturnoi Khimii (Issue-No. from 1981)'
_journal_page_first              573
_journal_page_last               577
_journal_volume                  18
_journal_year                    1977
_chemical_formula_sum            'I O Pr'
_chemical_name_systematic        'Pr O I'
_space_group_IT_number           129
_symmetry_space_group_name_Hall  'P 4ab 2ab -1ab'
_symmetry_space_group_name_H-M   'P 4/n m m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.086
_cell_length_b                   4.086
_cell_length_c                   9.162
_cell_volume                     152.963
_citation_journal_id_ASTM        ZSTKAI
_cod_data_source_file            Potapova_ZSTKAI_1977_144.cif
_cod_data_source_block           I1O1Pr1
_cod_original_cell_volume        152.9632
_cod_original_sg_symbol_Hall     '-P 4a 2a (x-1/4,y+1/4,z)'
_cod_original_formula_sum        'I1 O1 Pr1'
_cod_database_code               1530611
Hydrogen bonds in Na2 S (D2 O)9: Neutron diffraction, x-ray diffraction and vibrational spectroscopic studies
Preisinger, A.; Baumgartner, O.; Mereiter, K.; Heger, G.; Steidl, H.; Mikenda, W.; Inorganica Chimica Acta 57 (1982) 237–246; doi:

data_1530612
_publ_section_title
;
 Hydrogen bonds in Na2 S (D2 O)9: Neutron diffraction, x-ray diffraction
 and vibrational spectroscopic studies
;
_journal_name_full               'Inorganica Chimica Acta'
_journal_page_first              237
_journal_page_last               246
_journal_volume                  57
_journal_year                    1982
_chemical_formula_sum            'D18 Na2 O9 S'
_chemical_name_systematic        'Na2 S (D2 O)9'
_space_group_IT_number           95
_symmetry_space_group_name_Hall  'P 4cw 2c'
_symmetry_space_group_name_H-M   'P 43 2 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.337
_cell_length_b                   9.337
_cell_length_c                   12.783
_cell_volume                     1114.416
_citation_journal_id_ASTM        ICHAA3
_cod_data_source_file            Preisinger_ICHAA3_1982_722.cif
_cod_data_source_block           D18Na2O9S1
_cod_original_formula_sum        'D18 Na2 O9 S1'
_cod_database_code               1530612
Crystal structure of yttrium polonide
Prokin, E.S.; Ershova, Z.V.; Ermolaev, E.E.; Chebotarev, N.T.; Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy 11 (1975) 1230–1232; doi:

data_1530613
_publ_section_title
;
 Crystal structure of yttrium polonide
;
_journal_name_full
'Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy'
_journal_page_first              1230
_journal_page_last               1232
_journal_volume                  11
_journal_year                    1975
_chemical_formula_sum            'Po Y'
_chemical_name_systematic        'Y Po'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   6.251
_cell_length_b                   6.251
_cell_length_c                   6.251
_cell_volume                     244.258
_citation_journal_id_ASTM        IVNMAW
_cod_data_source_file            Prokin_IVNMAW_1975_198.cif
_cod_data_source_block           Po1Y1
_cod_original_cell_volume        244.2578
_cod_original_formula_sum        'Po1 Y1'
_cod_database_code               1530613
Titanium, zirconium and hafnium monopolonides.
Prokin, E.S.; Chebotarev, N.T.; Aksenov, B.S.; Ershova, Z.V.; Radiokhimiya 20 (1978) 684–686; doi:

data_1530614
_publ_section_title
;
 Titanium, zirconium and hafnium monopolonides.
;
_journal_name_full               Radiokhimiya
_journal_page_first              684
_journal_page_last               686
_journal_volume                  20
_journal_year                    1978
_chemical_formula_sum            'Po Ti'
_chemical_name_systematic        'Ti Po'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   3.992
_cell_length_b                   3.992
_cell_length_c                   6.569
_cell_volume                     90.659
_citation_journal_id_ASTM        RADKAU
_cod_data_source_file            Prokin_RADKAU_1978_175.cif
_cod_data_source_block           Po1Ti1
_cod_original_cell_volume        90.65901
_cod_original_formula_sum        'Po1 Ti1'
_cod_database_code               1530614
Titanium, zirconium and hafnium monopolonides.
Prokin, E.S.; Aksenov, B.S.; Ershova, Z.V.; Chebotarev, N.T.; Radiokhimiya 20 (1978) 684–686; doi:

data_1530615
_publ_section_title
;
 Titanium, zirconium and hafnium monopolonides.
;
_journal_name_full               Radiokhimiya
_journal_page_first              684
_journal_page_last               686
_journal_volume                  20
_journal_year                    1978
_chemical_formula_sum            'Po Zr'
_chemical_name_systematic        'Zr Po'
_space_group_IT_number           194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   4.031
_cell_length_b                   4.031
_cell_length_c                   6.907
_cell_volume                     97.195
_citation_journal_id_ASTM        RADKAU
_cod_data_source_file            Prokin_RADKAU_1978_185.cif
_cod_data_source_block           Po1Zr1
_cod_original_cell_volume        97.1954
_cod_original_formula_sum        'Po1 Zr1'
_cod_database_code               1530615